# Chapter 7. Highlights:

Save this PDF as:

Size: px
Start display at page:

## Transcription

1 Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true strain, strain exponent, and know the difference between elastic and plastic deformation.. Understand what a stress-strain curve is and what information it contains about materials properties. Be able to identify and/or calculate all the properties in #1 from a stress-strain curve, both in the elastic and plastic (before necking) regions. 3. Understand how the mechanical behavior of ceramics differs from that of metals. Be able to numerically manipulate the flexural strength and the effect of porosity on mechanical strength. 4. Understand how the mechanical behavior of polymers differs from that of metals. Understand and be able to numerically manipulate the viscoelastic modulus. Notes: Show Figures 7.1 to 7.4.

2 Define engineering stress and strain (tension and compression): Engineering stress F A Engineering strain ε l i - l l l l

3 For shear stress, Shear stress τ F A Shear strain γ tanθ ( θ is strain angle) As shown in Figure 7.4, and described in Equations 7.4a and 7.4b, an applied axial force can be geometrically decomposed into tensile and shear components. Stress-strain test: slowly increase stress and measure strain until the material fractures (show Figures 7., 7.3, 7.5, 7.1-1). These tests are usually performed in tension. In the linear portion of the curve, Hooke's law is obeyed, Eε. E is called the modulus of elasticity, or Young's modulus, and is a property of the material. The units of E are psi or MPa, remembering that PaN/m. Typical values for E are given in Table 7.1 for metals, ceramics and polymers.

4

5

6 A similar relationship can be written for compressive, shear, and torsional loads. For shear stress, τ G γ G is the shear modulus and is a property of the material. On an atomic scale, lengthening (compressing) a specimen during tensile (compressive) loading results in lengthening (shortening) of atomic bonds. Young's modulus is a measure of the resistance to separation of adjacent atoms. Youngs modulus df dr r Show Figure 7.7 and Table 7.1. High E- W and Ni, low E- Mg, Al, Au, Ag. Show Table 3.7. E can be different in different directions, and this reflects the different atomic densities in different planes and directions. When there is not a significant linear portion of an engineering stressstrain diagram, the secant and tangent modulus are sometimes employed. Show Figure 7.6. The tangent modulus is the slope of the stressstrain curve at one particular point, while the secant modulus is the slope of a secant drawn from the origin to a particular point on the stressstrain curve. By common sense, tensile strain in the z direction should yield compressive strain in the x and y directions. Show Figure 7.9. ε x ε y. Define Poisson's ratio υ ε ε y ν - x - ε z ε z υ for most metals, and is again a property of the material. It can be shown that G.4E for most metals. E G(1+ ν ) The following analogies illustrate the differences between the linear and nonlinear portions of a stress-strain curve:

7 Hooke's law Bonds stretched Elastic deformation No permanent damage Nonlinear -ε Bonds broken Plastic deformation Permanent damage Example Problem A cylindrical steel bar 1 mm in diameter is to be elastically deformed. Using the data in Table 7.1, determine the force needed to produce a reduction of 3x1-3 mm in the diameter. From Table 7.1, E 7 GPa and ν.3. We are given information about the desired radial strain: ε r 3 3x1 mm 4 3x1 1 mm This can be related to the axial strain by the definition of Poisson s ratio, eq. 7.8: ε z 4 3x1 3 ε r 1x1 υ.3 Now use Hooke s law, eq. 7.5, to determine the stress that must be applied: 3 ( 1x1 ).7GPa MPa Eε (7GPa) 7 From the definition of stress, eq. 7.3, F 6 π A 7 x1 Pa (.1m) 1.63x1 4 4 N Tensile Properties of Materials: Show a stress-strain curve, Figure 7.1. We will now digress for a while but eventually return to this figure and try to understand it and extract useful information. The linear portion of this curve undergoes elastic deformation (linear -ε), which disappears after the stress is removed. In other words, it is reversible. When the stress exceeds the linear portion of the stress-strain curve, permanent (irreversible) plastic deformation occurs. Plastic deformation Plastic deformation usually occurs near ε.5 for metals. When Hooke's law fails, the material undergoes plastic deformation. Show Figure 7.1. Either 7.1a or 7.1b can occur, usually 7.1a. Since plastic deformation involves atomic-level breaking of bonds and reforming of new ones, it is irreversible. We want to be able to define unambiguously when a material yields, when it is permanently damaged. Show Figure 7.1a, focusing on point P. This is the proportional limit, where the stress-strain curve deviates from linearity. But this is ambiguous.

8 Usually the stress-strain curve deviates from linearity quite gradually, so we need to define an arbitrary but universal definition of the elastic region. Starting from point, ε., draw a parallel line to the linear portion of the stress-strain curve. The stress at which this line intersects with the stress-strain curve is called the yield strength, y. This is one measure of a material's strength, its ability to resist plastic (permanent) deformation. In the case of Figure 7.1b the yield strength is the lower yield point. Show Figure The tensile strength is defined as the maximum stress prior to fracture. After M, "necking" occurs, the cross-sectional area shrinks abruptly. The ductility is defined as the % plastic deformation at fracture. Ductility A low ductility material is brittle. Show Figure l f - l l x1 Resilience is the capability of a material to absorb energy when it is deformed elastically. The modulus of resilience U r is ε y U r dε where ε y is the strain at fracture. Show Figure For linear stress-strain curve, U r 1 y ε y y E Toughness is the ability of a material to absorb energy up to fracture. It is defined by the same integral as U r above, but the upper limit of integration is now fracture instead of yielding. Show Table 7.3. High ductility corresponds somewhat with low strength. Example Problem For a given set of data, which I will not reproduce here, you should be able to: a) Create a plot of engineering stress versus engineering strain, b) determine the elastic modulus, c) determine the yield strength, d) determine the tensile strength, e) determine the ductility, and f) determine the modulus of resilience. a) The plots below were obtained by taking: F( N ) F( N ) ( Pa ) π π 3 D ( 1.8x1 m) F( N )

9 ε l i i l l l e8 Stress (Pa).e8 1.e8.e Strain b) The elastic modulus is taken as the slope of the linear portion of the curve. Looking at the nd plot, which focuses on the linear portion of the curve, take the average slope only from the 1 st four points. This yields: x1 Pa 1.173x1 Pa 1.795x1 Pa E ε x1 Pa.398 Taking the average of these 4 values yields E 5.88x1 1 Pa. c) On the nd plot, draw a line from ε. with a slope of E 5.88x1 1 Pa. The intersection of this line with the -ε curve gives y.8x1 8 Pa. d) From the 1 st plot, the maximum in is the tensile strength 3.7x1 8 Pa. e) From the 1 st plot, the strain at failure is about.145, subtract out the elastic strain (.5) to get the plastic strain of.14. Thus the ductility is 14%.

10 f) Determine the modulus of resilience from equation 7.14: U r y E Elastic recovery after plastic deformation: Show figure 7.17 and discuss. 8 (.8x1 Pa) (5.88x1 1 Pa) 6.67x1 5 Pa True Stress and Strain: True stress( T ) and true strain(ε T ) are defined similarly to engineering stress and strain. T F A i Force Instantaneous area ε l ln l T i l i is the instantaneous length If volume is conserved, then A i l i A l and T (1 + ε ) ε T ln (1 + ε ) The above two equations are only true until necking. After necking, true stress and true strain can only be

11 determined by actual measurements. Show Figure 7.16, where the true stress is corrected to account for nontensile components. For some metals, from the onset of plastic deformation to the point at which necking begins, the true stress is approximately: n T K ε T K and n, the strain hardening exponent, vary across different metals and alloys. Example Problem You are given that just prior to necking, (, ε) (35 MPa,.194) and (5 MPa,.96). What value of will produce ε.5. In order to use equation (7.19), we need to convert from engineering stress and strain to true stress and strain. From equations (7.18) 1 T (1+ ε ) MPa T (1+ ε ) 34 MPa 1 ε T ln(1+ ε ).1773 ε T ln(1+ ε ) ε T ln(1+ ε ).31 You need to use equation (7.19) to setup two equations with two unknowns. Taking the ln of both sides: ln(34 ln ln K + nlnε T MPa ) ln K + n ln(.593) T

12 ln(8.59 MPa ) ln K + n ln(.1773) Subtracting the nd from the 1 st ln n ln Substituting back into above: n.378 ln (8.59 MPa ) ln K + (.378) ln(.1773) ln K 6.91 or K 54 MPa Now find where ε T is.31: n T K ε T.378 T (54 MPa)(.31) MPa Convert back to engineering stress: T 1 + ε 36.3 MPa MPa Mechanical behavior: Ceramics Ceramic materials are less mechanically useful than metals because they are generally quite brittle. Their mechanical strength is not normally assessed by tensile stress-strain measurements. It is extremely difficult to prepare the proper sample geometry, the samples generally crack when gripped, and their strain at failure is too small to accurately measure. Show Figure For these reasons, the strength of ceramic materials is normally assessed by a traverse bending test. Show Figure The failure point is described by the flexural strength ( fs ), also known as the modulus of rupture( mr ). For rectangular cross sections, and for circular cross-sections: fs 3 F f L b d F f L π R fs 3

13

14 Example Problem A 3-point bending test is performed on Al O 3 with a circular cross-section of radius 3.5 mm. The specimen fractures at a load of 95 N when the support points are 5 mm apart. Consider a square sample of the same material with a square cross-section of 1mm on each edge. If the support points are 4 mm apart, at what load will the sample fracture? First, determine the flexural strength of this material from equation (7.b): fs F L 3 f (95 N )(5x1 m) 3.53x πr π (3.5x1 m) 8 Pa Now determine the failure force from equation (7.a): F bd 3 3 fs (1x1 m) 3 3L 3(4x1 (3.53x1 m) 8 Pa) 1,17 N Ceramic solids are often fabricated by compaction or foaming of ceramic particles. In this case, the ceramic solid may have considerable porosity, which degrades its strength. The modulus of elasticity (E) and the flexural strength ( fs ) depend on the volume fraction porosity (P) according to: ( 1 1.9P. P ) E E + 9 fs exp( np) where and n are experimental constants. Example Problem Using the data in Table 7., a) Determine the flexural strength of nonporous MgO assuming n 3.75 b) Calculate the volume fraction porosity when fs 6 MPa. a) Taking the ln of both sides of equation 7.: ln fs ln np From Table 7., fs 15MPa with 5% porosity, so ln(15 MPa ) ln (3.75)(.5) ln MPa

15 b) Rearranging the above equation: P ln ln fs n ln(6 MPa) P or 19vol.% Note that 5% porosity reduces fs by 17%, and 19% porosity reduces fs by 51%.

16 Mechanical behavior: Polymers Typical stress-strain diagrams for polymers are shown in Figure 7.. The behavior ranges from strong and brittle (curve A) to rubbery (curve C). The mechanical behavior of polymers is far more temperaturedependent than that of metals and polymers. Show Figure 7.4. Polymethyl methylacrylate behaves like a brittle metal at low temperature, but like an elastomer (rubber band) at low temperature. At intermediate temperatures, this polymer behaves like a viscoelastic material, which combines the behavior of a viscous and an elastic material. The most famous viscoelastic material is silly putty, which is intermediate between a liquid and a solid. Show Figure 7.6, which shows the strain behavior with time following instantaneous application of a load. Alternatively, one can study the mechanical behavior of a viscoelastic material at constant strain, in which case the stress that is initially applied will gradually decrease. Show Figure 7.7, which shows the stress as a function of time and temperature. How can we compare different materials?? One way is to choose an arbitrary time (1 sec is common) and define the relaxation modulus, E r (t), at that time: E r ( t) ( t) ε Remember that the value of E r (1) depends on the temperature. Show Figure 7.7 again.

17 Safety factor Engineering with a safety factor accounts for material variability, nonideal conditions, human error, etc. and is common engineering practice. The working stress ( w ) is reduced from the yield stress ( y ) by the safety factor (N) according to: The safety factor N is commonly taken as. y w N

### Introduction to Engineering Materials ENGR2000. Dr. Coates

Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed

### Outline. Tensile-Test Specimen and Machine. Stress-Strain Curve. Review of Mechanical Properties. Mechanical Behaviour

Tensile-Test Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress - true strain (flow curve) mechanical properties: - Resilience - Ductility - Toughness - Hardness A standard

### Stress-Strain Behavior

Stress-Strain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.

### Chapter 6: Mechanical Properties of Metals. Dr. Feras Fraige

Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness

### 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and

6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile

### MECE 3321 MECHANICS OF SOLIDS CHAPTER 3

MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.

### Mechanical properties 1 Elastic behaviour of materials

MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical

### EMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain - Axial Loading

MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain - Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain - Axial Loading Statics

### 4.MECHANICAL PROPERTIES OF MATERIALS

4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stress-strain diagram

### CHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS

CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a cross-sectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress

### UNIT I SIMPLE STRESSES AND STRAINS

Subject with Code : SM-1(15A01303) Year & Sem: II-B.Tech & I-Sem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES

### MECHANICS OF MATERIALS

Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:

### How materials work. Compression Tension Bending Torsion

Materials How materials work Compression Tension Bending Torsion Elemental material atoms: A. Composition a) Nucleus: protons (+), neutrons (0) b) Electrons (-) B. Neutral charge, i.e., # electrons = #

### Laboratory 4 Bending Test of Materials

Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective

### MATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?

MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition

### 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?

IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at

### Elastic Properties of Solid Materials. Notes based on those by James Irvine at

Elastic Properties of Solid Materials Notes based on those by James Irvine at www.antonine-education.co.uk Key Words Density, Elastic, Plastic, Stress, Strain, Young modulus We study how materials behave

### Mechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering

Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected

### Geology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)

Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties: - elastic modulii Outline of this Lecture 1. Uniaxial rock

### Lab Exercise #3: Torsion

Lab Exercise #3: Pre-lab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round

### Lecture 7, Foams, 3.054

Lecture 7, Foams, 3.054 Open-cell foams Stress-Strain curve: deformation and failure mechanisms Compression - 3 regimes - linear elastic - bending - stress plateau - cell collapse by buckling yielding

### Materials and Structures. Indian Institute of Technology Kanpur

Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional

### five Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture

ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS

### five Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture

ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS

### Structural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature

Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment Tinius-Olsen Lo-Torq Torsion Machine (figure

### Chapter 26 Elastic Properties of Materials

Chapter 26 Elastic Properties of Materials 26.1 Introduction... 1 26.2 Stress and Strain in Tension and Compression... 2 26.3 Shear Stress and Strain... 4 Example 26.1: Stretched wire... 5 26.4 Elastic

### ANSYS Mechanical Basic Structural Nonlinearities

Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria

### A concrete cylinder having a a diameter of of in. mm and elasticity. Stress and Strain: Stress and Strain: 0.

2011 earson Education, Inc., Upper Saddle River, NJ. ll rights reserved. This material is protected under all copyright laws as they currently 8 1. 3 1. concrete cylinder having a a diameter of of 6.00

### Design of a fastener based on negative Poisson's ratio foam adapted from

1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205-212 (1991).

### 6.37 Determine the modulus of resilience for each of the following alloys:

6.37 Determine the modulus of resilience for each of the following alloys: Yield Strength Material MPa psi Steel alloy 550 80,000 Brass alloy 350 50,750 Aluminum alloy 50 36,50 Titanium alloy 800 116,000

Fundamentals of Durability Page 1 Your single provider of solutions System simulation solutions 3D simulation solutions Test-based engineering solutions Engineering services - Deployment services Troubleshooting

### Experiment Two (2) Torsional testing of Circular Shafts

Experiment Two (2) Torsional testing of Circular Shafts Introduction: Torsion occurs when any shaft is subjected to a torque. This is true whether the shaft is rotating (such as drive shafts on engines,

### X has a higher value of the Young modulus. Y has a lower maximum tensile stress than X

Bulk Properties of Solids Old Exam Questions Q1. The diagram shows how the stress varies with strain for metal specimens X and Y which are different. Both specimens were stretched until they broke. Which

### CHAPTER 6: ULTIMATE LIMIT STATE

CHAPTER 6: ULTIMATE LIMIT STATE 6.1 GENERAL It shall be in accordance with JSCE Standard Specification (Design), 6.1. The collapse mechanism in statically indeterminate structures shall not be considered.

### Tuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE

1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & Free-Body Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for

### THE DETERMINATION OF FRACTURE STRENGTH FROM ULTIMATE TENSILE AND TRANSVERSE RUPTURE STRESSES

Powder Metallurgy Progress, Vol.3 (003), No 3 119 THE DETERMINATION OF FRACTURE STRENGTH FROM ULTIMATE TENSILE AND TRANSVERSE RUPTURE STRESSES A.S. Wronski, A.Cias Abstract It is well-recognized that the

### 1. Demonstrate that the minimum cation-to-anion radius ratio for a coordination number of 8 is

1. Demonstrate that the minimum cation-to-anion radius ratio for a coordination number of 8 is 0.732. This problem asks us to show that the minimum cation-to-anion radius ratio for a coordination number

### UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.

UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude

### 3. BEAMS: STRAIN, STRESS, DEFLECTIONS

3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets

### Chapter 12. Static Equilibrium and Elasticity

Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial

Name: Date: Solid Mechanics Homework nswers Please show all of your work, including which equations you are using, and circle your final answer. Be sure to include the units in your answers. 1. The yield

### Chapter 3. Load and Stress Analysis

Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3

### BME 207 Introduction to Biomechanics Spring 2017

April 7, 2017 UNIVERSITY OF RHODE ISAND Department of Electrical, Computer and Biomedical Engineering BE 207 Introduction to Biomechanics Spring 2017 Homework 7 Problem 14.3 in the textbook. In addition

### TINIUS OLSEN Testing Machine Co., Inc.

Interpretation of Stress-Strain Curves and Mechanical Properties of Materials Tinius Olsen has prepared this general introduction to the interpretation of stress-strain curves for the benefit of those

### Pharmaceutical compounding I Colloidal and Surface-Chemical Aspects of Dosage Forms Dr. rer. nat. Rebaz H. Ali

University of Sulaimani School of Pharmacy Dept. of Pharmaceutics Pharmaceutical Compounding Pharmaceutical compounding I Colloidal and Surface-Chemical Aspects of Dosage Forms Dr. rer. nat. Rebaz H. Ali

### FCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering

FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001-015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress

### MSE 383, Unit 3-3. Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept.

Dynamic Mechanical Behavior MSE 383, Unit 3-3 Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept. Scope Why DMA & TTS? DMA Dynamic Mechanical Behavior (DMA) Superposition Principles

### Flexure: Behavior and Nominal Strength of Beam Sections

4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kip-in.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015

### External Work. When a force F undergoes a displacement dx in the same direction i as the force, the work done is

Structure Analysis I Chapter 9 Deflection Energy Method External Work Energy Method When a force F undergoes a displacement dx in the same direction i as the force, the work done is du e = F dx If the

### 1 Stress and Strain. Introduction

1 Stress and Strain Introduction This book is concerned with the mechanical behavior of materials. The term mechanical behavior refers to the response of materials to forces. Under load, a material may

### Elastic-Plastic Fracture Mechanics. Professor S. Suresh

Elastic-Plastic Fracture Mechanics Professor S. Suresh Elastic Plastic Fracture Previously, we have analyzed problems in which the plastic zone was small compared to the specimen dimensions (small scale

### Mechanics of Materials MENG 270 Fall 2003 Exam 3 Time allowed: 90min. Q.1(a) Q.1 (b) Q.2 Q.3 Q.4 Total

Mechanics of Materials MENG 70 Fall 00 Eam Time allowed: 90min Name. Computer No. Q.(a) Q. (b) Q. Q. Q.4 Total Problem No. (a) [5Points] An air vessel is 500 mm average diameter and 0 mm thickness, the

### Chapter 8. Shear and Diagonal Tension

Chapter 8. and Diagonal Tension 8.1. READING ASSIGNMENT Text Chapter 4; Sections 4.1-4.5 Code Chapter 11; Sections 11.1.1, 11.3, 11.5.1, 11.5.3, 11.5.4, 11.5.5.1, and 11.5.6 8.2. INTRODUCTION OF SHEAR

### The Frictional Regime

The Frictional Regime Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 1/25/2016 10:08 AM We Discuss The Frictional Regime Processes of Brittle Deformation

### 22 Which of the following correctly defines the terms stress, strain and Young modulus? stress strain Young modulus

PhysicsndMathsTutor.com Which of the following correctly defines the terms stress, strain and Young modulus? 97/1/M/J/ stress strain Young modulus () x (area) (extension) x (original length) (stress) /

### Symmetric Bending of Beams

Symmetric Bending of Beams beam is any long structural member on which loads act perpendicular to the longitudinal axis. Learning objectives Understand the theory, its limitations and its applications

### Introduction to Fracture

Introduction to Fracture Introduction Design of a component Yielding Strength Deflection Stiffness Buckling critical load Fatigue Stress and Strain based Vibration Resonance Impact High strain rates Fracture

### MASSACHUSETTS INSTITUTE OF TECHNOLOGY DEPARTMENT OF MATERIALS SCIENCE AND ENGINEERING CAMBRIDGE, MASSACHUSETTS 02139

MASSACHUSES INSIUE OF ECHNOLOGY DEPARMEN OF MAERIALS SCIENCE AND ENGINEERING CAMBRIDGE, MASSACHUSES 02139 3.22 MECHANICAL PROPERIES OF MAERIALS PROBLEM SE 5 SOLUIONS 1. (Hertzber 6.2) If it takes 300 seconds

### Strain-Based Design Model for FRP-Confined Concrete Columns

SP-230 57 Strain-Based Design Model for FRP-Confined Concrete Columns by N. Saenz and C.P. Pantelides Synopsis: A constitutive strain-based confinement model is developed herein for circular concrete columns

### CONSTITUTIVE RELATIONS FOR LINEAR ELASTIC SOLIDS

Chapter 9 CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS Figure 9.1: Hooke memorial window, St. Helen s, Bishopsgate, City of London 211 212 CHAPTR 9. CONSTITUTIV RLATIONS FOR LINAR LASTIC SOLIDS 9.1 Mechanical

### 5.2 The Response of Real Materials

5.2 The Response of Real Materials The constitutive equation as introduced in the previous section. The means by hich the constitutive equation is determined is by carrying out experimental tests on the

### MECH 401 Mechanical Design Applications

MECH 401 Mechanical Design Applications Dr. M. O Malley Master Notes Spring 008 Dr. D. M. McStravick Rice University Updates HW 1 due Thursday (1-17-08) Last time Introduction Units Reliability engineering

### Seismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design

Seismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design Elmer E. Marx, Alaska Department of Transportation and Public Facilities Michael Keever, California Department

### Lecture 2: Deformation in the crust and the mantle. Read KK&V chapter 2.10

Lecture 2: Deformation in the crust and the mantle Read KK&V chapter 2.10 Tectonic plates What are the structure and composi1on of tectonic plates? Crust, mantle, and lithosphere Crust relatively light

### Bending and Shear in Beams

Bending and Shear in Beams Lecture 3 5 th October 017 Contents Lecture 3 What reinforcement is needed to resist M Ed? Bending/ Flexure Section analysis, singly and doubly reinforced Tension reinforcement,

### Outline. Organization. Stresses in Beams

Stresses in Beams B the end of this lesson, ou should be able to: Calculate the maimum stress in a beam undergoing a bending moment 1 Outline Curvature Normal Strain Normal Stress Neutral is Moment of

### BTECH MECHANICAL PRINCIPLES AND APPLICATIONS. Level 3 Unit 5

BTECH MECHANICAL PRINCIPLES AND APPLICATIONS Level 3 Unit 5 FORCES AS VECTORS Vectors have a magnitude (amount) and a direction. Forces are vectors FORCES AS VECTORS (2 FORCES) Forces F1 and F2 are in

### Brittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm

Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd

### Fracture Behavior. Section

Section 6 Fracture Behavior In January 1943 the one-day old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and

### Spherical Pressure Vessels

Spherical Pressure Vessels Pressure vessels are closed structures containing liquids or gases under essure. Examples include tanks, pipes, essurized cabins, etc. Shell structures : When essure vessels

### A Critical Plane-energy Model for Multiaxial Fatigue Life Prediction. of Homogeneous and Heterogeneous Materials. Haoyang Wei

A Critical Plane-energy Model for Multiaxial Fatigue Life Prediction of Homogeneous and Heterogeneous Materials by Haoyang Wei A Thesis Presented in Partial Fulfillment of the Requirements for the Degree

### CHEM-C2410: Materials Science from Microstructures to Properties Composites: basic principles

CHEM-C2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and

### Chapter 13 ELASTIC PROPERTIES OF MATERIALS

Physics Including Human Applications 280 Chapter 13 ELASTIC PROPERTIES OF MATERIALS GOALS When you have mastered the contents of this chapter, you will be able to achieve the following goals: Definitions

### 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.

Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation

### Rheology and the Lithosphere

Rheology and the Lithosphere Processes in Structural Geology & Tectonics Ben van der Pluijm WW Norton+Authors, unless noted otherwise 3/8/2017 16:51 We Discuss Rheology and the Lithosphere What is rheology?

### Prof. B V S Viswanadham, Department of Civil Engineering, IIT Bombay

56 Module 4: Lecture 7 on Stress-strain relationship and Shear strength of soils Contents Stress state, Mohr s circle analysis and Pole, Principal stressspace, Stress pathsin p-q space; Mohr-Coulomb failure

### 3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,

3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it

### Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity",

Reference material Reference books: Y.C. Fung, "Foundations of Solid Mechanics", Prentice Hall R. Hill, "The mathematical theory of plasticity", Oxford University Press, Oxford. J. Lubliner, "Plasticity

### Fatigue Problems Solution

Fatigue Problems Solution Problem 1. (a) Given the values of σ m (7 MPa) and σ a (1 MPa) we are asked t o compute σ max and σ min. From Equation 1 Or, σ m σ max + σ min 7 MPa σ max + σ min 14 MPa Furthermore,

### Therefore, for all members designed according to ACI 318 Code, f s =f y at failure, and the nominal strength is given by:

5.11. Under-reinforced Beams (Read Sect. 3.4b oour text) We want the reinforced concrete beams to fail in tension because is not a sudden failure. Therefore, following Figure 5.3, you have to make sure

### DEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8 - PART 3 PROVISIONS

DEFORMATION CAPACITY OF OLDER RC SHEAR WALLS: EXPERIMENTAL ASSESSMENT AND COMPARISON WITH EUROCODE 8 - PART 3 PROVISIONS Konstantinos CHRISTIDIS 1, Emmanouil VOUGIOUKAS 2 and Konstantinos TREZOS 3 ABSTRACT

### Testing and Analysis

Testing and Analysis Testing Elastomers for Hyperelastic Material Models in Finite Element Analysis 2.6 2.4 2.2 2.0 1.8 1.6 1.4 Biaxial Extension Simple Tension Figure 1, A Typical Final Data Set for Input

### Rheology. What is rheology? From the root work rheo- Current: flow. Greek: rhein, to flow (river) Like rheostat flow of current

Rheology What is rheology? From the root work rheo- Current: flow Greek: rhein, to flow (river) Like rheostat flow of current Rheology What physical properties control deformation? - Rock type - Temperature

### MECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola

MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the

Failure from static loading Topics Quiz /1/07 Failures from static loading Reading Chapter 5 Homework HW 3 due /1 HW 4 due /8 What is Failure? Failure any change in a machine part which makes it unable

### Question Figure shows the strain-stress curve for a given material. What are (a) Young s modulus and (b) approximate yield strength for this material?

Question. A steel wire of length 4.7 m and cross-sectional area 3.0 x 10-5 m 2 stretches by the same amount as a copper wire of length 3.5 m and cross-sectional area of 4.0 x 10-5 m 2 under a given load.

### EFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS

EFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS Atsuhiko MACHIDA And Khairy H ABDELKAREEM SUMMARY Nonlinear D FEM was utilized to carry out inelastic

### Materials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.

Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie

### NE 125 L. Title Page

NE 125 L Title Page Name: Rajesh Swaminathan ID Number: 20194189 Partners Names: Clayton Szata 20193839 Sarvesh Varma 20203153 Experiment Number: 1 Experiment: Date Experiment was Started: Date Experiment

### Continuum Mechanics. Continuum Mechanics and Constitutive Equations

Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform

### Question 1. Ignore bottom surface. Solution: Design variables: X = (R, H) Objective function: maximize volume, πr 2 H OR Minimize, f(x) = πr 2 H

Question 1 (Problem 2.3 of rora s Introduction to Optimum Design): Design a beer mug, shown in fig, to hold as much beer as possible. The height and radius of the mug should be not more than 20 cm. The

### Torsion of Solid Sections. Introduction

Introduction Torque is a common load in aircraft structures In torsion of circular sections, shear strain is a linear function of radial distance Plane sections are assumed to rotate as rigid bodies These

### Task 1 - Material Testing of Bionax Pipe and Joints

Task 1 - Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 604-534-8631 Fax: 604-534-7616

### Determine the resultant internal loadings acting on the cross section at C of the beam shown in Fig. 1 4a.

E X M P L E 1.1 Determine the resultant internal loadings acting on the cross section at of the beam shown in Fig. 1 a. 70 N/m m 6 m Fig. 1 Support Reactions. This problem can be solved in the most direct

### CIVL222 STRENGTH OF MATERIALS. Chapter 6. Torsion

CIVL222 STRENGTH OF MATERIALS Chapter 6 Torsion Definition Torque is a moment that tends to twist a member about its longitudinal axis. Slender members subjected to a twisting load are said to be in torsion.

### Experiment: Torsion Test Expected Duration: 1.25 Hours

Course: Higher Diploma in Civil Engineering Unit: Structural Analysis I Experiment: Expected Duration: 1.25 Hours Objective: 1. To determine the shear modulus of the metal specimens. 2. To determine the

### Strength of Material. Shear Strain. Dr. Attaullah Shah

Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume

### SERVICEABILITY OF BEAMS AND ONE-WAY SLABS

CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach - Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONE-WAY SLABS A. J. Clark School of Engineering Department of Civil